# Plasmonic silicon Schottky photodetectors: The physics ...

### Transcript of Plasmonic silicon Schottky photodetectors: The physics ...

APL Photonics 2, 026103 (2017); https://doi.org/10.1063/1.4973537 2, 026103

© 2017 Author(s).

Plasmonic silicon Schottky photodetectors:The physics behind graphene enhancedinternal photoemission Cite as: APL Photonics 2, 026103 (2017); https://doi.org/10.1063/1.4973537Submitted: 17 September 2016 . Accepted: 20 December 2016 . Published Online: 12 January 2017

Uriel Levy, Meir Grajower, P. A. D. Gonçalves , N. Asger Mortensen , and Jacob B. Khurgin

COLLECTIONS

This paper was selected as Featured

ARTICLES YOU MAY BE INTERESTED IN

The physics and chemistry of the Schottky barrier heightApplied Physics Reviews 1, 011304 (2014); https://doi.org/10.1063/1.4858400

Metal-semiconductor-metal photodetectors based on graphene/p-type silicon SchottkyjunctionsApplied Physics Letters 102, 013110 (2013); https://doi.org/10.1063/1.4773992

Schottky contact surface-plasmon detector integrated with an asymmetric metal stripewaveguideApplied Physics Letters 95, 021104 (2009); https://doi.org/10.1063/1.3171937

APL PHOTONICS 2, 026103 (2017)

Plasmonic silicon Schottky photodetectors: The physicsbehind graphene enhanced internal photoemission

Uriel Levy,1 Meir Grajower,1 P. A. D. Goncalves,2,3 N. Asger Mortensen,2,3

and Jacob B. Khurgin4,a1Department of Applied Physics, The Benin School of Engineering, The Center for Nanoscienceand Nanotechnology, The Hebrew University of Jerusalem, Jerusalem, Israel2Department of Photonics Engineering, Technical University of Denmark,DK-2800 Kongens Lyngby, Denmark3Center for Nanostructured Graphene, Technical University of Denmark,DK-2800 Kongens Lyngby, Denmark4Department of Electrical and Computer Engineering, Johns Hopkins University, Baltimore,Maryland 21218, USA

(Received 17 September 2016; accepted 20 December 2016; published online 12 January 2017)

Recent experiments have shown that the plasmonic assisted internal photoemissionfrom a metal to silicon can be significantly enhanced by introducing a monolayerof graphene between the two media. This is despite the limited absorption in amonolayer of undoped graphene (∼πα = 2.3%). Here we propose a physical modelwhere surface plasmon polaritons enhance the absorption in a single-layer grapheneby enhancing the field along the interface. The relatively long relaxation time ingraphene allows for multiple attempts for the carrier to overcome the Schottkybarrier and penetrate into the semiconductor. Interface disorder is crucial to over-come the momentum mismatch in the internal photoemission process. Our resultsshow that quantum efficiencies in the range of few tens of percent are obtain-able under reasonable experimental assumptions. This insight may pave the wayfor the implementation of compact, high efficiency silicon based detectors for thetelecom range and beyond. © 2017 Author(s). All article content, except where oth-erwise noted, is licensed under a Creative Commons Attribution (CC BY) license(http://creativecommons.org/licenses/by/4.0/). [http://dx.doi.org/10.1063/1.4973537]

In recent years, plasmonic enhanced silicon detectors based on internal photoemission (IPE)across the metal-silicon Schottky barrier have been demonstrated and shown to be useful in thedetection of telecom band (1300-1600 nm)—beyond the detection capability of conventional siliconphotodiodes and photoconductors. Both guided wave and free space configurations were imple-mented.1–13 While such demonstrations open new opportunities for CMOS compatible nanophotonicsand nanoplasmonics, the quantum efficiency of such detectors still falls well short off the commer-cially available InGaAs detectors. This is primarily due to the low transmission probability of electronstraversing the metal-silicon interface, combined with fast thermalization (∼10 fs) of photo-excitedhot electrons in the metal.14

Recently, it has been shown that the insertion of a graphene monolayer in between the metaland the semiconductor greatly enhances the internal quantum efficiency to about 7%.15 While alarge variety of photodetectors based on two dimensional materials have been demonstrated,16 mostof them are based on mechanisms which are different from the internal photoemission effect and todate, the graphene-metal-silicon photodetector seems to be a leading candidate for CMOS compatibleinternal photoemission detection in the telecom window. The observed enhancement in quantumefficiency makes photodetectors based on internal photoemission highly relevant for a variety ofapplications, e.g., chip scale optical communications. The reasons for such a significant enhancement

aAuthor to whom correspondence should be addressed. Electronic mail: [email protected]

2378-0967/2017/2(2)/026103/6 2, 026103-1 © Author(s) 2017

026103-2 Levy et al. APL Photonics 2, 026103 (2017)

are not yet fully understood, and in general the transport of hot carriers (electrons and holes) betweentwo-dimensional and three-dimensional materials is still an active topic of research.

In this work, we address this issue by developing a phenomenological model which explainsthe physics behind graphene-silicon internal photoemission based detectors. The model not onlycaptures the latest findings but also provides guidelines for obtaining efficient internal photoemissionprocesses, in terms of surface roughness, field confinement, and momentum matching.

The structure that is considered in this paper is that of a graphene monolayer, sandwiched betweena metal and a semiconductor, as depicted in Fig. 1.

In the context of photodetectors based on internal photoemission from a metal to a semiconductor,graphene may offer the advantage of high absorption the 2D layer provides, while at the same timeit can be placed right at the metal-semiconductor interface. This high absorption is attributed to thedirect interband transition. This is in contrast to typical metals, in which absorption is based on freecarriers, and must involve a mediator such as phonons or defects to provide momentum conservation.As a result, the graphene monolayer is capable of absorbing the light within a propagation length offew tens of microns and can be considered as a significant absorption mechanism, co-existing withthe Ohmic damping in the metal. This can be shown by the following expression for the dispersionrelation of the plasmonic mode with and without (by making σ→ 0) the presence of the intermediategraphene layer (see, e.g., Refs. 17 and 18 and references therein)

εsi√q2 − εsiω2/c2

+εM√

q2 − εMω2/c2=

σ

iε0ω, (1)

where εM = 1 −ω2

p

ω∗(ω+iγ) is the Drude-like dielectric function of the metal, εsi = 12 denotes the rel-ative permittivity of silicon, ω is the angular frequency, q is the in-plane wave vector, and σ is theoptical conductivity of graphene. Neglecting doping, this conductivity is entirely due to direct inter-band transitions, i.e., σ = e2/4~= cπαε0. Due to the small magnitude of the fine structure constant,α ∼ 1/137, we perturbatively treat the effect of graphene on the SPP dispersion relation: to the lowestorder, we find the complex valued shift in the wavevector to be ∆q∝ α. In the next step we calculatethe enhanced absorption Γ= Im(∆q)

Im(q0) of the surface plasmon polariton (SPP) due to the presence of

graphene. For low frequencies, the result is given by Γ' 2πα ω2

γωp, where γ andωp are the damping

rate and the plasma frequency of the metal, respectively. By substituting typical values for gold atan operation frequency of 0.8 eV (telecom), one obtains up to 20% enhancement, depending on thespecific choice of damping factor. Therefore, the relative absorption in graphene with respect to thetotal absorption is given by Γ/ (1 + Γ) and the SPP propagation length is now L = L0

1+Γ , where L0 isthe SPP propagation length in the absence of graphene. With the above estimate, about 17% of thelight is being absorbed in the graphene layer over a length of ∼30 µm.

It should be noted that operating closer to the surface plasmon resonance, there is even a regimewith slow light enhancement (not captured by the perturbative expansion). Another alternative for

FIG. 1. Schematic diagram illustrating the geometry of the studied structure.

026103-3 Levy et al. APL Photonics 2, 026103 (2017)

enhancing the absorption in graphene is by patterning the metallic layer on top with subwavelengthstructures, as discussed, e.g., in Ref. 19.

Since the transition in graphene is vertical, the energy of all the hot carriers is always ~ω/2 abovethe Dirac point (Fig. 2(a)) in clear contrast to the absorption in the metal where photo-generatedcarriers have broad energy distribution. Assuming this value is above the Schottky barrier, the elec-tron has sufficient energy and will cross the barrier provided that lateral momentum is preserved(Fig. 2(b)). We further note that in graphene, being a 2D material, any hot carrier is at the boundarywith silicon.

In metals, the above-mentioned scenario is different for two major reasons: (a)—the plasmonicmode decays about 10 nm into the metal and thus the probability of the hot carrier to be generatedat the boundary is finite. As a result, some of the hot carriers will experience thermalization and willnot make it to the barrier. (b)—the hot carriers have a distribution of energies. Some of the carriershave sufficient energy to cross the barrier, while others do not.

Another important issue relates to the relaxation dynamics of hot electrons. Thermalization timein graphene, which is determined by electron-electron scattering, is on the time scale of 100 fs, whiletypical values for metals are significantly shorter, in the 10 fs range. This allows for multiple attemptsfor a hot electron to be transported across the Schottky barrier into the silicon as they are “bounced”back and forth in the atomically thin layer of graphene. This process further enhances the probabilityof internal photoemission.

Before providing a more detailed analysis, let us consider the impact of having all the absorptionoccurring in a monolayer. We conceptually represent the monolayer as a quantum well with a thicknessa∼ 3 Å and assume that a photoexcited carrier is travelling back and forth in the well, with a velocityof v= π~/m0a. Therefore, the round trip time is τrt = 2a/v= 2a2m/π~= ~ (π~2/2ma2)−1 which isroughly 0.5 fs.

Assigning a transmission probability T to the transition from graphene to either silicon or metal,the effective emission time becomes τem = τrt/(2T ). At the same time the thermalization time of hotcarriers is τth ∼ 100 fs (for recent ultrafast spectroscopy experiments of hot electrons in graphene see,e.g., Ref. 20). Then, the quantum efficiency of the emission into the silicon is given by η = 1

2τth

τth+τem

= 12

τthτth+τrt /2T . Assuming a relatively low transmission value of 0.1%, which is a characteristic value

of metal-semiconductor interfaces,14 one obtains a quantum efficiency in excess of 10%! This hugeenhancement is entirely due the multiple attempts for transmission. Clearly, the large absorptionin a single-layer of graphene plays a pivotal role in such an enhancement, as every photo-excitedcarrier is always not further than ∼3 Å from the graphene-silicon interface. It should be stated thatthe relatively long thermalization time of free carriers in graphene (∼100 fs, as opposed to ∼10 fs

FIG. 2. (a) Electron energy band diagram of graphene, near the Dirac point. The horizontal dashed line is associated withthe Fermi level under weak doping conditions (not to scale). For generality, we have slightly shifted the Fermi energy levelfrom the Dirac point. (b) Schematic illustration of the internal photoemission process from the metal through the grapheneand to the semiconductor. Photon energy is assumed to be larger than the Schottky barrier. The black solid line represents ahot electron that was transported to silicon through the barrier, while the red dashed line represents a hot electron that wasreflected from the barrier. The blue line denotes the conduction band level in the silicon.

026103-4 Levy et al. APL Photonics 2, 026103 (2017)

in metal), combined with the use of a waveguide configuration which allows the efficient absorp-tion of light over relatively short propagation distance absorption, is pivotal in obtaining such highefficiencies.

Obviously, this rough prediction depends upon the value of T which reflects the character ofatomic wavefunctions in the semiconductor and in the graphene, and also relies critically on the in-plane momentum conservation as depicted in Fig. 3 where the projection of the cubic Brillouin zoneof Si onto the (kx, ky) plane is shown superimposed onto the hexagonal Brillouin zone of graphene,with the principal axis rotated by an arbitrary angle which cannot be predicted during fabrication.The key issue is that the photo-excited carriers (both holes and electrons) in graphene are located inthe vicinity of the K points of graphene. The magnitude of the lateral wavevector of these carriers is

about K = 1.71 Å−1

, and their energy is comparable to either the top of the valence band of a p-typesilicon, located at the center of the Brillouin zone (kv ∼ 0), or the bottom of the conduction band,located at one of the six valleys along the 100 directions. Two of these valleys (pink circles) have an

in-plane wavevector (kc ∼ 0) while the other four (pink ellipsoids) are located at (kc ∼ 1 Å−1

).Therefore, the momentum mismatch involved in the transmission of a carrier from the graphene

to the silicon is fairly large. If the photo-excited carrier is a hole going into the Γ valley of Si, then

the mismatch is on the scale of δkKΓ ∼ 1.7 Å−1

, while for the photo-excited electrons going into the

X valley of Si the mismatch is about δkKX ∼ 0.9 Å−1

.However, this dire situation can be relaxed if one considers the possibility of the Umklapp

process,21 where momentum conservation, shown in Fig. 3, is written as ~K =~kc/v + ~G, where ~G is oneof the reciprocal lattice vectors. For example, ~G=

[2πa , 2π

a , 2πa

]in silicon has an absolute value of its

projection onto the xy plane (shown in Fig. 3 as an orange arrow) of−−−→|Gxy | = 1.63 Å

−1, which is close

to the K point in graphene. As one can see from Fig. 3 with the help of the Umklapp process, theoverall mismatch between the states in graphene and silicon ∆k | | is significantly reduced, yet it is stillnot zero, especially when one considers the inevitable randomness of the relative orientation of the

FIG. 3. Brillouin zones of Si (red) and graphene (blue) in the xy-plane. Because of the violation of momentum conservation,the hot electrons (holes) photo-generated in the vicinity of K-points of graphene (light blue circles) cannot be transferredto the minima (maxima) of the conduction (valence) band located near X (Γ) points and shown as pink ellipsoids (circles).They can, however, be transferred to the energy minimum (maximum) of the second Brillouin zone of Si-circle Γ2Si via theUmklapp process enabled by the lattice vector G. For generality, we have slightly rotated the graphene lattice with respect tothe silicon lattice. In fact, while this rotation can take any value in the range of 0◦–360◦, owing to the six-fold symmetry ofthe hexagonal lattice, it is sufficient to describe the angle between 0◦ and 30◦.

026103-5 Levy et al. APL Photonics 2, 026103 (2017)

lattices. However, this small momentum mismatch can be mitigated by the disorder and roughnessalways present at the interface, as was observed, e.g., in the internal photoemission from the metalto the silicon in a plasmonic waveguide Schottky photodetector.8 We now discuss this scenario ingreater detail.

The coupling between graphene and silicon can be described by the Hamiltonian Hcoup

= 〈ΨG |H |Ψsi〉, corresponding to the scale of few eV. This Hamiltonian has a constant value H0

augmented by the disorder term Vd (x, y), given by Vd (x, y)=!

F(kx, ky)ei(kxx+kyy)dkxdky which

obviously is a random function but with a well-defined power spectrum |F(kx, ky)|2 ≡ ��F(k‖

) ��2

= π−1ΛV20 e−k2

‖Λ2

, where V20 is the power of the coupling integral variations and Λ is the correlation

length.According to the Fermi’s golden rule, we can now write the rate of transfer from a given state

in graphene with energy Egr above the Schottky barrier to a state in the silicon with an energy Esi

separated by the wavevector ∆k‖ as

<(∆k‖

)=

2π~

��F(∆k‖

) ��2a

2Lδ(Egr − Esi

(∆k‖

)), (2)

where L is the extent of the Si wavefunctions in the direction normal to the plane used for normalizationof these wavefunctions. This term will be cancelled once the integration over kz takes place in Eq. (3).Next we need to perform the summation over all the states in the silicon having the same k | | . Usingthe effective mass approximation, the delta-function in Eq. (2) becomes

δ *,E −~2k2

‖

2m∗−~2k2

z

2m∗+-=

m∗

~2kzδ *

,kz −

√2m∗E

~2− k2‖+-

. (3)

And thus

R (K)=2π~

aL

∫ √2m∗E2

~2

02πk‖dk‖ ��F

(K − k‖

) ��2∫ ∞

0

m∗

~2kzδ *

,kz −

√2m∗E

~2− k2‖+-

dkz ×L2π

, (4)

where K is wavevector of the state in graphene, roughly equal to the K-point. By integrating over kz,one obtains

R (K)=2π~

m∗a

~2

12

∫ 2m∗E~2

0

dk2‖√

2m∗E~2 − k2

‖

��F(K − k‖

) ��2 ≈���F

(⟨∆k2‖

⟩) ���2 π

~

m∗a

~2

√2m∗E

~2

∫ 1

0

dx√

1 − x

=V2

0

~

m∗Λ2

~2

√2m∗a2E

~2e−

⟨∆k2‖

⟩Λ2

. (5)

To further proceed, we should now estimate the transition rate using a reasonable parameter. The firstenergy level of our fictitious quantum well is given by ~2/2m∗a2 ∼ 3 eV whereas a typical energy forthe electron in the silicon is estimated to be E = 1 eV (this value is obtained by assuming a reasonableSchottky Barrier of 0.3 eV and using the photon energy at the wavelength of interest around 1.5 µm,

corresponding to ~ω/2= 0.4 eV). In this way, we obtain√

2m∗a2E~2 ' 0.2.

Next, we make V0 = 0.1 eV and Λ≈ 10 Å , so that m∗Λ2

~2 = 6.5 eV−1 and thereby arriving at

R (K)≈ 2 × 1013e−100⟨∆k2‖

⟩s−1, (6)

where ∆k‖ is given in units of Å−1

. The quantum efficiency can be estimated as simply the ratioη ∼Rτth/(Rτth + R′τth + 1), where R’ is the rate of transfer of carriers from graphene to the metal.

This rate is small because the Fermi wavevector in gold is kF ∼ 1.2 Å−1<K . Hence once again the

process of transfer from K states in graphene into the metal has Umklapp character. Therefore, for10% efficiency assuming thermalization time of 100 fs, we need R∼ 1012 s−1 which requires a very

reasonable momentum mismatch of about ∆k‖ = 0.17 Å−1

(this corresponds, e.g., to rotation by about9.7◦ between the projected Brillouin zones of graphene and silicon; see Fig. 3).

In summary, we have presented a heuristic model which provides a possible explanation forthe recently observed enhancement of internal photoemission efficiency from a metal to silicon.

026103-6 Levy et al. APL Photonics 2, 026103 (2017)

Based on our model, the photo-generated hot electrons generated at the graphene layer can havemultiple attempts of penetrating into the silicon due to the long thermalization time with respectto the round trip time of carriers in the monolayer, and thus having higher probability of escapinginto the semiconductor and be collected as a useful photocurrent. We argue that the momentummismatch between graphene and silicon can be partially overcom with the aid of Umklapp processes.This, combined with inevitable interface roughness, can provide efficiencies in excess of 10%, whichmakes graphene a viable candidate for enhancing Schottky barrier sub-bandgap photodetector. As afinal note, it is interesting to observe the role of SPP in enhancing the interaction of light with grapheneto such an extent that the low absorption of graphene monolayer is still sufficient for achieving decentphotocurrents, owing to the field enhancement at the interface and the use of guided surface modes.

We deeply acknowledge Ilya Goykhman for fruitful discussions and for providing experimen-tal data. The work was supported by the National Science Foundation (Grant No. 1507749), theUnited States—Israel Binational Science Foundation (BSF), the Danish National Research Foun-dation Center for Nanostructured Graphene, Project No. DNRF103, and the Danish InternationalNetwork Programme with Israel, Danish Agency for Science, Technology and Innovation (GrantNos. 1370-00124B and 4070-00158B).

1 A. Akbari and P. Berini, “Schottky contact surface-plasmon detector integrated with an asymmetric metal stripe waveguide,”Appl. Phys. Lett. 95, 21104 (2009).

2 P. Berini, “Surface plasmon photodetectors and their applications,” Laser Photonics Rev. 8, 197–220 (2014).3 M. L. Brongersma, N. J. Halas, and P. Nordlander, “Plasmon-induced hot carrier science and technology,” Nat. Nanotechnol.

10, 25–34 (2015).4 H. Chalabi, D. Schoen, and M. L. Brongersma, “Hot-electron photodetection with a plasmonic nanostripe antenna,” Nano

Lett. 14, 1374–1380 (2014).5 M. W. Knight et al., “Embedding plasmonic nanostructure diodes enhances hot electron emission,” Nano Lett. 13, 1687–1692

(2013).6 M. W. Knight, H. Sobhani, P. Nordlander, and N. J. Halas, “Photodetection with active optical antennas,” Science 332,

702–704 (2011).7 B. Desiatov et al., “Plasmonic enhanced silicon pyramids for internal photoemission Schottky detectors in the near-infrared

regime,” Optica 2, 335–338 (2015).8 I. Goykhman, B. Desiatov, J. Khurgin, J. Shappir, and U. Levy, “Waveguide based compact silicon Schottky photodetector

with enhanced responsivity in the telecom spectral band,” Opt. Express 20, 28594–28602 (2012).9 I. Goykhman, B. Desiatov, J. Khurgin, J. Shappir, and U. Levy, “Locally oxidized silicon surface-plasmon Schottky detector

for telecom regime,” Nano Lett. 11, 2219–2224 (2011).10 M. Casalino, G. Coppola, M. Iodice, I. Rendina, and L. Sirleto, “Critically coupled silicon Fabry-Perot photodetectors based

on the internal photoemission effect at 1550 nm,” Opt. Express 20, 12599 (2012).11 W. Li and J. Valentine, “Metamaterial perfect absorber based hot electron photodetection,” Nano Lett. 14, 3510–3514

(2014).12 P. Berini, A. Olivieri, and C. Chen, “Thin Au surface plasmon waveguide Schottky detectors on p-Si,” Nanotechnology 23,

444011 (2012).13 Z. Han et al., “On-Chip detection of radiation guided by dielectric-loaded plasmonic waveguides,” Nano Lett. 15, 476–480

(2015).14 I. Goykhman, B. Desiatov, and, J. Shappir, “Model for quantum efficiency of guided mode plasmonic enhanced silicon

Schottky detectors,” preprint arXiv:1401.2624 (2014).15 I. Goykhman et al., “On-chip integrated, silicon�graphene plasmonic Schottky photodetector with high responsivity and

avalanche photogain,” Nano Lett. 16, 3005–3013 (2016).16 F. H. L. Koppens et al., “Photodetectors based on graphene, other two-dimensional materials and hybrid systems,” Nat.

Nanotechnol. 9, 780 (2014).17 P. A. D. Goncalves and N. M. R. Peres, An Introduction to Graphene Plasmonics (World Scientific, 2016).18 S. Xiao, X. Zhu, B.-H. Li, and N. A. Mortensen, “Graphene-plasmon polaritons: From fundamental properties to potential

applications,” Front. Phys. 11, 117801 (2016).19 M. Hashemi, M. H. Farzad, N.A. Mortensen, and S. Xiao, “Enhanced absorption of graphene in the visible region by use

of plasmonic nanostructures,” J. Opt. 15, 55003 (2013).20 Z. Mics et al., “Thermodynamic picture of ultrafast charge transport in graphene,” Nat. Commun. 6, 7655 (2015).21 N. W. Ashcroft and N. D. Mermin, Solid State Physics (Holt, Rinehart and Winston, New York, 1976).